Quantum Hall Effect on Top and Bottom Surface States of Topological

Insulator (Bi1−xSbx)2Te 3 Films

R. Yoshimi1*, A. Tsukazaki2,3, Y. Kozuka1, J. Falson1, K. S. Takahashi4, J. G. Checkelsky1,

N. Nagaosa1,4, M. Kawasaki1,4 and Y. Tokura1,4

1 Department of Applied Physics and Quantum-Phase Electronics Center (QPEC),

University of Tokyo, Tokyo 113-8656, Japan

2 Institute for Materials Research, Tohoku University, Sendai 980-8577, Japan

3 PRESTO, Japan Science and Technology Agency (JST), Chiyoda-ku, Tokyo 102-0075,

Japan

４ RIKEN Center for Emergent Matter Science (CEMS), Wako 351-0198, Japan.

* Corresponding author: [email protected]

1

The three-dimensional (3D) topological insulator (TI) is a novel state of matter as characterized by two-dimensional (2D) metallic Dirac states on its surface1-4. Bi-based

chalcogenides such as Bi2Se3, Bi2Te 3, Sb2Te 3 and their combined/mixed compounds

like Bi2Se2Te and (Bi1−xSbx)2Te 3 are typical members of 3D-TIs which have been intensively studied in forms of bulk single crystals and thin films to verify the topological nature of the surface states5-12. Here, we report the realization of the

Quantum Hall effect (QHE) on the surface Dirac states in (Bi1−xSbx)2Te 3 films (x = 0.84 and 0.88). With electrostatic gate-tuning of the Fermi level in the bulk band gap under magnetic fields, the quantum Hall states with filling factor ν = ± 1 are resolved with

2 quantized Hall resistance of Ryx = ± h/e and zero longitudinal resistance, owing to chiral edge modes at top/bottom surface Dirac states. Furthermore, the appearance of

a ν = 0 state (σxy = 0) reflects a pseudo-spin Hall insulator state when the Fermi level is tuned in between the energy levels of the non-degenerate top and bottom surface

Dirac points. The observation of the QHE in 3D TI films may pave a way toward

TI-based electronics.

Quantum transport in Dirac electron systems has been attracting much attention for the half-integer quantum Hall effect (QHE), as typically observed in graphene13, 14. The

2 recently discovered topological insulator (TI) possesses metallic Dirac states on the edge or surface of an insulating bulk1-4. With the application of a magnetic field (B) the unique features of Dirac bands may be exemplified via the formation of Landau levels (LLs). The

QHE is the hallmark of dissipationless topological quantum transport originating from one-dimensional chiral edge modes driven by cyclotron motion of two-dimensional (2D) electrons. Unlike the case of graphene which has a four-fold degeneracy originating from the spin and valley degrees of freedom, the degeneracy is completely lifted in the spin-polarized Dirac state of 2D and 3D TIs. For such 3D TI films the top and bottom surfaces support surface states with opposite spin-momentum locked modes when top and bottom surfaces are regarded as two independent systems. Such a helicity degree of freedom in real space can be viewed as the pseudo-spin variable and is hence expected to

yield a new quantum state via tuning of surface magnetism and/or Fermi level (EF) that is applicable to quantum computation functions15-17. Although intensive research has been carried out for bulk crystals, thin films, and field-effect devices5-12, parasitic bulk conduction and/or disorder in the devices continues to hamper efforts to resolve quantum transport characteristics of the Dirac states on chalcogenide 3D TIs surfaces. The most venerable example of the QHE with least bulk conduction has been achieved in 70nm

3 strained HgTe film18. Compared to the HgTe system, 3D-TIs of Bi-chalcogenides such as

Bi2Se2Te and (Bi1−xSbx)2Te3 have a good potential for exploring the Dirac surface states with wide controllability of transport parameters (resistivity, carrier type and density) and band parameters (energy gap, position of Dirac point and Fermi velocity) by changing the compositions19, 20.

In this work, we report transport measurements on 3D TI thin films of (Bi1−xSbx)2Te3 (x

= 0.84 and 0.88; both 8 nm thick). Using molecular beam epitaxy19 and insulating InP (111)

substrates, the EF of as-grown film was tuned near to the bulk band edge by precisely controlling the Bi/Sb composition ratio in the film19, 20. Films were then fabricated into

photolithography defined gated Hall-bar devices to allow electrostatic tuning of EF. A cross-sectional schematic of the device structure and the top-view image are shown in Figs.

1a and 1b, respectively. The device consists of Hall bar defined by Ar ion-milling, and an

atomic-layer-deposited AlOx insulator isolates Ti/Au top gate with electron-beam evaporated Ti/Au electrodes (see Methods). The magnetotransport measurements were carried out in a dilution refrigerator by low-frequency (3 Hz) lock-in technique with low excitation current of 1 nA to suppress heating.

First, device operation was examined at B = 0 T. Figure 1c shows the electric field

4 effect controlled conductivity σxx of the x = 0.84 film as a function of top gate voltage VG with changing temperature. The minimum conductance of roughly 2 e2/h (e: the elemental

charge, h: Planck constant) is observed at VG = −1.7 V. On both sides of this minimum, σxx

shows a linear but asymmetric increase with increasing or decreasing VG. The weak

temperature dependence of σxx for a wide range of VG is characteristic of the gapless nature of Dirac states under finite disorder21. Thus we ascribe the conductivity of this TI film below 1 K to the Dirac surface states with a small contribution from bulk conduction. To

verify the ambipolar nature of the device, the longitudinal and transverse resistance Rxx and

Ryx as a function of VG at B = 3 T were measured (Fig. 1d). As expected, this results in a

sign change of Ryx at a certain VG which we hereafter define as the gate voltage

corresponding to EF being located at the charge neutral point (CNP), VCNP. This point

coincides closely with the VG at which Rxx reaches a maximum. At the VCNP, the Hall effects

from top and bottom surface states appear to cancel, resulting in Ryx ~ 0, although electron-rich and hole-rich puddles are thought to still exist, as in the case of graphene22. To capture the essence of the observed phenomena, we hereafter take the working hypothesis

that EF shifts equally on top and bottom states which in turn retain the difference in energy

position. The inverse of Hall coefficient 1/RH is shown in Fig. 1e, which would be

5 proportional to 2D charge carrier density n2D = 1/eRH, in the simplest case. Asymmetric

behavior of 1/RH between positive and negative VG regions with respect to VCNP is in accord

with the asymmetric σxx behavior at zero magnetic field as shown in Fig. 1c. The more

efficient increase in σxx with electron accumulation (positive VG) is often observed in

8-12 ambipolar TI transistors and may be related to the difference in vF (Fermi velocity) above and below the Dirac point19. In addition, the proximity of the Dirac point to the valence band edge needs to be taken into account for the present thin film system; in most

of the negative region of VG − VCNP, EF must go inside the valence band in which doped holes appears to be fully localized at low temperatures below 1 K, as argued later.

With applying higher magnetic field of B = 14 T, clear signatures of QHE are revealed

in the temperature dependence of Rxx and Ryx, as shown in Figs. 2a-d for the x = 0.84 film

and in Figs. 2e-h for the x = 0.88 film. We first focus on the results of the x = 0.84 film. Rxx

increases steeply with lowering the temperature for VG corresponding to the CNP, while

decreases rapidly toward zero in the both sides at higher and lower VG. Concomitantly to

2 the decrease in Rxx, Ryx reaches the values of quantum resistance ± h/e = ± 25.8 kΩ and

forms plateaus in VG at T = 40 mK. This correspondence between the rapidly declining Rxx

2 value and the quantized Ryx plateaus at ± h/e are distinct evidence for QHE at Landau

6 filling factor ν = ± 1, respectively, as schematically shown in Fig. 2i. The LL splitting

2 energy of Dirac dispersion (En) is given by n = ||2)sgn( h F eBvnnE , where n is the LL index.

Using the data of Rxx and Ryx, σxy and σxx as functions of VG − VCNP for the x = 0.84

2 film are plotted in Figs. 2c and 2d. Again, the Hall plateaus at σxy = ± e /h as well as

minima of σxx approaching zero (black triangles) are observed and are indicative of the

QHE with ν = ± 1. In this plot, however, two additional features are to be noted. The first

is an unexpectedly wide σxy plateau and thermally activated behavior of σxx for the ν = +1

2 (σxy = e /h) state in the corresponding VG – VCNP (negative) region. As already noted in the

VG asymmetric change of σxx (Fig. 1c) in the negative region of VG − VCNP , i.e. hole-doping,

EF readily reaches the valence band top. The energy position of Dirac point of the x = 0.84 film lies by at most 30 meV above the valence band top, while the LL splitting between n =

0 and n = −1 levels amounts to 70 meV at 14 T, according to resonant tunneling

spectroscopy on similarly grown thin films of (Bi1−xSbx)2Te3 (Ref. 19). From the

consideration of the Fermi velocity of Dirac cone, the VG − VCNP value at which the EF reaches the valence band top is estimated to be around −1.5 V or an even a smaller absolute

value. Therefore, in the VG − VCNP region where the quantum Hall plateau or its precursor is

7 observed, the EF locating between n = 0 and n = −1 LLs of the surface state is close to or already buried in the valence band, as schematically shown in Fig. 2i. While the doped but

localized holes in the valence band may hardly contribute to transport, i.e. σxy (bulk) << σxy

(surface), the relative EF shift with negatively sweeping VG − VCNP becomes much slower as compared with the positive sweep case owing to the dominant density of states of the valence band. This explains a wider plateau region for ν = +1 in the hole-doping side, contrary to the normal behavior of electron accumulation side, ν = −1.

The second notable feature in Fig. 2c is the emergence of the ν = 0 state around VG =

VCNP, as seen in the step of σxy and (finite) minimum in σxx as functions of VG − VCNP. This state is more clearly resolved in the x = 0.88 film, as shown in Figs. 2e-h, on which we focus hereafter. In a similar manner to the x = 0.84 film, the x = 0.88 film also shows with

lowering temperature divergent behavior of Rxx around VG = VCNP, while approaching zero

around VG − VCNP = −1.5 V. The Ryx reaches 25.8 kΩ around VG − VCNP = −1.5 V forming

the ν = +1 quantum Hall state, while in the electron doping regime Ryx reaches −20 kΩ, short of the quantized value. The failure to form the fully quantized ν = −1 state is perhaps related to the disorder of the surface Dirac state which is induced by the compositional/structural disorder of the as-grown film and cannot be overcome by gate

8 tuning.

Nevertheless, the ν = 0 feature is clearly resolved for the x = 0.88 film, as shown in the

2 VG dependence of σxy (Fig. 2g) calculated from Rxx and Ryx. In addition to the σxy = e /h (ν

= +1) plateau, a plateau at σxy = 0 appears at around VG = VCNP. The plateau broadening

2 occurs via centering at σxy = 0.5 e /h as the isosbestic point with elevating temperature. In

accordance with the plateaus in σxy, σxx takes a minima at ν = +1 and 0, as shown in Fig. 2h.

Here, we can consider the contribution of the both top and bottom surface Dirac states to

this quantization of σxy, as schematically shown in Fig. 2j. At the ν = +1 (ν = −1) state, the

both top and bottom surfaces are accumulated by holes (electrons) with EF being located between n = 0 and n = −1 (n = +1) LLs, giving rise to the chiral edge channel. In contrast, we assign the ν = 0 state to the gapping of the chiral edge channel as the cancelation of the

contributions to σxy from the top and bottom surface states with ν = ± 1/2, when EF locates in between the energy levels of the top and bottom surface Dirac points (n = 0 levels), as shown in Fig. 2j. This ν = 0 state can hence be viewed as a pseudo-spin Hall insulator, if we consider the top and bottom degree of freedom as the pseudo-spin variable. Such an observation of a zero conductance plateau has been reported also in disordered graphene under very high magnetic field23-26 and analyzed theoretically27, as well as in the 2D TIs,

9 the quantum wells of HgTe28 and InAs/GaSb29. From the analyses shown in the following,

we propose here that the major origin for the presence of σxy = 0 is more like the energy difference of the top/bottom Dirac points rather than other effect such as electron-hole puddles in composition inhomogeneity.

To further discuss the characteristics of these QH states, we investigate the B

dependence of σxy (Figs. 3a and b). The analysis of the plateau width against VG determines the phase diagram as shown in Figs. 3c and d. The plateau edges are determined from the

second derivative of σxy with respective to VG (see Supplementary Information (SI)), while

the plateau transition points between ν = 0 and ν = ± 1 are defined here by σxy = ± 1/2 e2/h. The plateau shrinks with decreasing B for the ν = −1 state of the x = 0.84 film (Fig.

3a). However, the ν = +1 state for the both films appears to be rather robust with reducing

VG (doping more holes), since EF positions already below the top of the valence band,

perhaps for VG − VCNP < −1.5 V. On the other hand, the ν = 0 plateau is only weakly dependent on B, although the plateau width is wider for x = 0.88 than for x = 0.84. The observation of ν = 0 requires the condition that the Fermi level is located in between the energy levels of the top and bottom surface Dirac points (Fig. 2j). From the Hall data in the

relatively high positive VG − VCNP region (electron-doping) shown in Fig. 1e, we can know

10 the relation between the sum of the top and bottom Dirac electron density versus VG − VCNP.

2 Then, with the values of the ν = 0 plateau width between the σxy = ± 0.5 e /h points (δVG

5 19 ~0.9 V and 1.4 V; see Figs. 3c and d) and the Fermi velocity (vF ~ 5 × 10 m/s) , we can

estimate the energy difference (δEDP) between the Dirac points at the top and bottom surface states to be ~ 50 meV and ~70 meV for the x = 0.84 and x = 0.88 film, respectively

(see SI). These values should be compared with a much larger band gap energy (~ 250

meV). The energy difference δEDP is, however, considerably larger than a Zeeman shift (~9 meV at 14 T)19, which rationalizes the above analysis with ignoring the Zeeman shift of the n = 0 LL. While the reason why the two films (x = 0.84 and 0.88) show such a difference in

δEDP is not clear at the moment, we speculate that the monolayer buffer layer of Sb2Te3 (x =

1.0) used for the growth of the x = 0.88 film (see SI) may cause the considerably higher

energy position of the Dirac point at the bottom surface. Incidentally, for the region of |VG −

VCNP| < 1/2 δVG, electron accumulation at the top surface and hole accumulation at the bottom surface should coexist. This may naturally explain the observed (Fig. 1e and see

also SI) deviation from the linear relationship between 1/RH and VG − VCNP as well as the

extrema of 1/RH observed at around ± 1/2δVG.

Figure 4 summarizes the flow of conductivity tensor (σxy, σxx) plotted with the two

11 experimental subparameters (T and VG) at 14 T. With decreasing T, the flow in (σxy, σxx)

2 2 tends to converge toward either of (σxy, σxx) = (−e /h, 0), (0, 0) or (e /h, 0) at high magnetic field (e.g. 14 T), which corresponds to ν = −1, 0 and +1 QH state, respectively. Incipient convergence to ν = 0 is discerned for the x = 0.84 film, while the ν = −1 state is not discernible for the x = 0.88 film. Among these three QH states, the unstable fixed point

2 appears to lie on the line of σxy = ± 0.5 e /h (approximately with the critical σxx value of ~

2 0.5 e /h) which corresponds to the crossing of EF at the n = 0 LL (or Dirac point) of the bottom and top surface state (see Fig. 2j), respectively30.

In conclusion, we have successfully observed the QHE at ν = ± 1 and 0 states in

three-dimensional TI thin films of (Bi1−xSbx)2Te3 (x = 0.84 and 0.88). Due to a considerable difference of the Dirac point (or n = 0 LL) energies of the top and bottom surfaces of the

thin film, the ν = 0 state observed at σxy = 0 is interpreted as a pseudo-spin Hall insulator with the top/bottom degree of freedom as the pseudo-spin. Further studies on non-local transport in mesoscopic structures will open the door to dissipationless topological-edge electronics based on the 3D topological insulators.

12

Methods

Thin films of (Bi1−xSbx)2Te3 (x = 0.84 and 0.88) were fabricated by molecular beam epitaxy (MBE) on semi-insulating InP (111) substrate. The Bi/Sb composition ratio was calibrated by the beam equivalent pressure of Bi and Sb, namely 8 × 10−7 Pa and 4.2 × 10−6

Pa for x = 0.84 and 6 × 10−7 Pa and 4.4 × 10−6 Pa for x = 0.88. The Te flux was over-supplied with the Te / (Bi + Sb) ratio kept at about 20. The substrate temperature was

200°C and the growth rate was about 0.2 nm/min. Fabrication procedures for the x = 0.84 and 0.88 films are slightly different at the initial growth on InP surfaces. We grew the 0.84 film with supplying Te and (Bi + Sb) from the initial stage. For the x = 0.88 film, we started

with supplying Te and Sb for a monolayer growth of Sb2Te3 buffer layer followed by Bi

shutter opening. This difference may be an origin of the larger energy gap δEDP of the Dirac points between the top and bottom surfaces (Fig. 2j) for the x=0.88 film. After the epitaxial growth of 8nm-thick thin films, those were annealed in-situ at 380°C to make the surface

smoother. AlOx capping layer was deposited at room temperature with an atomic layer deposition system immediately after the discharge of the samples from MBE. This process turned out to be effective to protect the surface from the degradation. The device structure was defined by subsequent photolithography and Ar ion-milling processes. Ohmic-contact

13 electrodes and top gate electrode were Ti/Au deposited with an e-beam evaporator. Here, ion-milling was performed under 45 degree tilt condition on a rotating stage, resulting in the ramped side edge as schematically shown in Fig. 1a. This ensured the electrical contact to the top and bottom of the film.

Reference

1. Hasan, M. Z. & Kane, C. L. Colloquium: Topological insulators. Rev. Mod. Phys. 82,

3045 (2010).

2. Kane, C. L. & Mele, E. J. Z2 Topological Order and the Quantum Spin Hall Effect. Phys.

Rev. Lett. 95, 146802 (2005).

3. Fu, L., Kane, C. L. & Mele, E. J. Topological insulators in three dimensions. Phys. Rev.

Lett. 98, 106803 (2007).

4. Hsieh, D. et al. A tunable topological insulator in the spin helical Dirac transport regime.

Nature 460, 1101-1105 (2009).

5. Analytis, J. G., et al. Two-dimensional surface state in the quantum limit of a

topological insulator Nature Phys. 6, 960-964 (2010).

6. Qu, D. X., Hor, Y. S., Xiong, J., Cava, R. J. & Ong, N. P. Quantum Oscillations and Hall

14

Anomaly of Surface States in the Topological Insulator Bi2Te3. Science 329, 821-824

(2010).

7. Taskin, A. A., Ren, Z., Sasaki, S., Segawa, K. & Ando, Y. Observation of Dirac Holes

and Electrons in a Topological Insulator. Phys. Rev. Lett. 107, 016801 (2011).

8. Checkelsky, J. G., Hor, Y. S., Cava, R. J. & Ong, N. P. Bulk Band Gap and Surface State

Conduction Observed in Voltage-Tuned Crystals of the Topological Insulator Bi2Se3.

Phys. Rev. Lett. 106, 196801 (2011).

9. Steinberg, H., Laloë, J. –B., Fatemi, V., Moodera, J. S. & Jarillo-Herrero, P. Electrically

tunable surface-to-bulk coherent coupling in topological insulator thin films Phys. Rev.

B 84, 233101 (2011).

10. Kong, D., et al. Ambipolar field effect in the ternary topological insulator (BixSb1-x)2Te3

by composition tuning. Nature Nanotech. 6, 705-709 (2011).

11. Kim, D., et al. Surface conduction of topological Dirac electrons in bulk insulating

Bi2Se3. Nature Phys. 8, 459-463 (2012).

12. Yang, F., et al. Top gating of epitaxial (Bi1-xSbx)2Te3 topological insulator thin films.

Appl. Phys. Lett. 104, 161614 (2014).

13. Novoselov, K. S., et al. Two-dimensional gas of massless Dirac fermions in graphene.

15

Nature 438, 197-200 (2005).

14. Zhang, Y., Tan, Y. -W., Stormer, H. L. & Kim, P. Experimental observation of the

quantum Hall effect and Berry’s phase in graphene. Nature 438, 201-204 (2005).

15. Yu., R., et al. Quantized Anomalous Hall Effect in Magnetic Topological Insulators.

Science 329, 61-64 (2010).

16. Chang, C. –Z., et al. Experimental Observation of the Quantum Anomalous Hall Effect

in a Magnetic Topological Insulator. Science 340, 167-170 (2013).

17. Wang, J., Lian, B., Zhang, H. & Zhang, S. –C. Anomalous Edge Transport in the

Quantum Anomalous Hall State. Phys. Rev. Lett. 111, 086803 (2013).

18. Brüne, C., et al. Quantum Hall Effect from the Topological Surface States of Strained

Bulk HgTe. Phys. Rev. Lett. 106, 126803 (2011).

19. Yoshimi, R., et al. Dirac electron states formed at the heterointerface between a

topological insulator and a conventional semiconductor. Nature Mater. 13, 253-257

(2014).

20. Zhang, J., et al. Band structure engineering in (Bi1−xSbx)2Te3 ternary topological

insulators. Nature Commun. 2, 574 (2012).

21. Bolotin, K. I., Sikes, K. J., Hone, J., Stormer, H. L. & Kim, P. Temperature-Dependent

16

Transport in Suspended Graphene. Phys. Rev. Lett. 101, 096802 (2008).

22. Martin, J., et al. Observation of electron-hole puddles in graphene using a scanning

single-electron transistor. Nature Phys. 4, 144-148 (2008).

23. Abanin, D. A., et al. Dissipative Quantum Hall Effect in Graphene near the Dirac Point.

Phys. Rev. Lett. 98, 196806 (2007).

24. Checkelsky, J. G., Li, L. & Ong, N. P. Zero-Energy State in Graphene in a High

Magnetic Field. Phys. Rev. Lett. 100, 206801 (2008).

25. Giesbers, A. J. M., et al. Gap opening in the zeroth Landau level of graphene. Phys. Rev.

B 80, 201403(R) (2009).

26. Zhao, Y., C-Zimansky, P., Ghahari, F. & Kim, P. Magnetoresistance Measurement of

Graphene at the Charge Neutrality Point. Phys. Rev.Lett. 108, 106804 (2012).

27. Das Sarma, S. & Yang, K. The enigma of the ν = 0 quantum Hall effect in graphene.

Solid State Commun. 149, 1502-1506 (2009).

28. Büttner, B., et al. Single valley Dirac fermions in zero-gap HgTe quantum wells. Nature

Phys. 7, 418-422 (2011).

29. Nichele, F., et al. Insulating State and Giant Nonlocal Response in an InAs/GaSb

Quantum Well in the Quantum Hall Regime. Phys. Rev. Lett. 112, 036802 (2014).

17

30. Nomura, K. & Nagaosa, N. Surface-Quantized Anomalous Hall Current and the

Magnetoelectric Effect in Magnetically Disordered Topological Insulators. Phys. Rev.

Lett. 106, 166802 (2011).

Acknowledgements

R. Y. is supported by the Japan Society for the Promotion of Science (JSPS) through a research fellowship for young scientists. This research was supported by the Japan Society for the Promotion of Science through the Funding Program for World-Leading Innovative

R & D on Science and Technology (FIRST Program) on “Quantum Science on Strong

Correlation” initiated by the Council for Science and Technology Policy and by JSPS

Grant-in-Aid for Scientific Research(S) No.24224009 and 24226002. This work was carried out by joint research of the Cryogenic Research Center, the University of Tokyo.

Author contributions

R. Y. performed thin films growth and device fabrication. R.Y., Y. K. and J. F. performed the low temperature transport measurements. R. Y. analyzed the data and wrote the manuscript with contributions from all authors. A. T., K. S. T., J. G. C., M. K. and Y. T.

18 jointly discussed the results and guided the project. Y. T. conceived and coordinated the project.

Competing Financial Interests

The authors declare no competing financial interests.

Figure Legends

Figure 1 | Gating of topological insulator (Bi0.16Sb0.84)2Te 3 thin film. a, b,

Cross-sectional schematic and top-view photograph of a Hall-bar device. Broken line in (b)

indicates the position for (a). c, Top gate voltage VG dependence of longitudinal

conductance σxx at various temperatures. d, e, Effective gate voltage (VG − VCNP)

dependence of longitudinal and transverse resistance (Rxx and Ryx) and inverse of Hall

coefficient 1/RH under magnetic field B = 3 T at temperature T = 40 mK. The VG for the

charge neutral point (CNP), VCNP, is defined at the gate voltage where Ryx is crossing zero.

Figure 2 | Observation of the quantum Hall effect. a, b, e and f, Effective gate voltage

VG − VCNP dependence of Rxx and Ryx at various temperatures of T = 40-700 mK with application of magnetic field B = 14 T for the x = 0.84 (a, b) and x = 0.88 (e, f) films of

19

(Bi1−xSbx)2Te3. c, d, e and h, Effective gate voltage VG − VCNP dependence of σxx and σxy at various temperatures of T = 40 - 700 mK with application of magnetic field B = 14 T for

the x = 0.84 and x = 0.88 films of (Bi1−xSbx)2Te3 as deduced from the corresponding Rxx and

Ryx data. Triangles in (d) and (h) show the dips of σxx. i, Schematics of the Landau levels

(LLs) of the surface state of (Bi1−xSbx)2Te3 (x = 0.8-0.9) thin film in case of the degenerate top and bottom surface states. At a high field, e.g. 14 T, the n = −1 LL of the surface state

locates below the top of the valence band. When the Fermi energy (EF) is tuned between the

LLs, the quantum Hall state with index ν emerges. j, Schematics of the LLs of the top and bottom surface states in case the n = 0 (Dirac point) energy is different between the two surfaces.

Figure 3 | Magnetic field dependence of Hall plateaus. a, b, σxy at T = 40 mK under

various B as a function of effective gate voltage VG − VCNP for the x = 0.84 (a) and x = 0.88

(b) films. Traces for lower magnetic fields are each vertically offset by e2/h. Dotted lines

2 represent the plateau transitions as defined at σxy = ± 0.5 e /h. c, d, Quantized σxy phase diagram for the ν = +1, 0 and −1 (blue, green and red shaded, respectively) states associated with the plateau edges (filled squares) and the plateau transition point (filled

2 circles) defined at σxy = ± 0.5 e /h in the plane of magnetic field and VG − VCNP. The

20 plateau edges are determined by the second-order VG derivative of σxy (see SI).

Figure 4 | Flows of σxy and σxx. (σxy, σxx) are displayed with the two experimental

subparameters (T and VG). Each line connecting between points represents the flow

behavior of (σxy, σxx) with lowering temperature from 700 mK to 40 mK at the specific

value of VG at B = 14 T. The flows direct from upper to lower with decreasing temperature.

21

22

23

24

25

Supplementary Information for

Quantum Hall Effect on Top and Bottom Surface States of Topological Insulator

(Bi1−xSbx)2Te 3 Films

R. Yoshimi, A. Tsukazaki, Y. Kozuka, J. Falson, K. S. Takahashi, J. G. Checkelsky,

N. Nagaosa, M. Kawasaki and Y. Tokura

1. Measurement configuration Low temperature transport measurements were performed in a dilution refrigerator with a superconducting magnet employing a lock-in technique at a low frequency (~ 3 Hz) and with a low excitation current (~ 1 nA). In the measurement circuit shown in Fig. S1. A series resistance of 1 GΩ was introduced to maintain a constant current condition that was confirmed by the signal from the lock-in amplifier that measured the current fed through the sample. We stress that all of the displayed data in the Figures in main text are the raw data under each condition without any (anti)symmetrization procedure. We did observe negligible asymmetry under positive and negative magnetic fields.

Fig. S1 Measurement configurations with an AC excitation.

26

2. Charge neutral point in the device (x = 0.88) Transport characteristics for the device (x = 0.88) at B = 0 and 3 T are shown in Fig. S2.

VG dependence of σxx at B = 0 T presents similar trend to that in the device (x = 0.84) shown in Fig. 1c, exhibiting weak temperature dependence. It is noted that the minimum conductance was observed at around VG = 1 V, indicating that the device (x = 0.88) presented here has originally p-type charge carriers, while the device (x = 0.84) presented in main text has n-type conduction. With applying B = 3 T, we obtained ambipolar behavior with a peak in Rxx and a zero-crossing in Ryx. Contrary to the case of x = 0.84 device which has no Sb2Te3 buffer layer (see Fig. 1d in the main text), these two bias voltages differ slightly. Since we observe this difference only when a monolayer Sb2Te3 buffer is employed, we conclude that the difference in bias voltages is originating from the energy difference of the top and bottom surface states as depicted in the insets of Figs. S2b and S2c. At the bias voltage of Ryx = 0, electrons and holes exist on the top and bottom surface, respectively. Since the total conductivity is the sum of those at top and bottom surfaces, bias voltage at

Rxx maximum (conductivity minimum) does not correspond to that at Ryx = 0 owing to the mobility difference between electrons and holes. The energy difference between the two

Dirac points at the top and bottom surface states is estimated to be δEDP ~70 meV (see next section). We define VCNP for the device (x = 0.88) as the VG at the zero-crossing point in Ryx.

27

Fig. S2 (a) Top gate voltage (VG) dependence of longitudinal conductance σxx at various temperatures for the x = 0.88 device. The crossing bias position of two linear broken lines may be considered as the charge neutral point (CNP). However, the VG is slightly shifted from the VG giving CNP defined by Hall measurements. (b), (c) Effective gate voltage

(VG-VCNP) dependence of longitudinal and transverse resistance (Rxx and Ryx) and inverse of

Hall coefficient 1/RH under a magnetic field B = 3 T at a temperature T = 40 mK. VCNP is defined at the VG where Ryx changes its sign. The inset schematics in (b) illustrate the Fermi level position between the Dirac points of the top and bottom surface states, representing the CNP. Right (left) inset in (c) indicates the Fermi level position that allows electron (hole) occupation on both surface states.

28

3. Energy scales in the band alignment. To depict the relationship of Dirac dispersions on the top and bottom surface states shown in Fig. 2j, we deduce the energy difference of Dirac points (δEDP) from the difference in the gate voltages (δVG) of 1.4 V giving the plateau transitions from ν = 0 to neighboring ν = ± 1 states indicated by dotted lines and black circles in Fig. 3d of the main text for the x = 0.88 device. In order to convert δVG to the change in charge carrier density

δn2D, we assumed δn2D e = Ceff δVG, where Ceff is the effective capacitance. Ceff is deduced 11 −2 −1 as 5 × 10 cm V from the linear part of 1/RH vs. (VG – VCNP) relation shown in Fig. S2c. 11 −2 Then δn2D is estimated as 7 × 10 cm . We adopted here the electron accumulation side for fitting, since overlap of valence band may give error in the estimation in hole accumulation side. 2 Assuming Dirac k-linear dispersion, i.e., E = h vFk and n = k /4π (where n is the carrier density on the single Dirac cone, vF is Fermi velocity and k is Fermi wave number), δn2D 5 can be converted to δEDP. We took vF ~ 5 × 10 m/s as an averaged value of those of the electron and the hole in (Bi0.12Sb0.88)2Te3 (1,2) and obtained δEDP ~70 meV for the x = 0.88 device. The similar procedure was adopted for the estimate of δEDP of the x = 0.84 device; from the value of δVG = 0.9V (see Fig. 3c), we obtain δEDP ~ 50 meV. The δVG value is in good agreement with the difference in VG giving maxima in |Ryx| shown in Fig. S2c (x = 0.88) and Fig. 1e (x = 0.84). In between these maxima, electrons and holes coexist in the two Dirac states and the contribution to Ryx cancels each other. When the Fermi level moves across the Dirac points, only electrons (holes) contribute to Ryx, giving maximum in

|Ryx|.

29

4. Determination of the plateau edge in Fig. 3c and 3d. The plateau edges represented by the solid squares in Figs. 3c and 3d in main text were defined from the second derivative of σxy with respect to the VG as shown in Fig. S3. Under the magnetic field larger than 7 T, peaks and dips (lower triangles) appear as indicated, which correspond to the inflection points of σxy. Below 3T, no significant feature is observed.

Fig. S3 Second derivative of σxy with respect to the effective gate voltage VG − VCNP at various magnetic fields for (a) x = 0.84 and (b) x = 0.88 devices. The colors of triangles correspond to those of the data plot in Fig. 3c and 3d.

30

5. Magnetic field dependence of Rxx and Ryx towards the QH state in the device

Figures S4 shows the magnetic field dependence of Rxx and Ryx at T = 40 mK. VG − VCNP was tuned at the position to observe the largest Ryx values. With increasing magnetic field, 2 Ryx linearly increases and bends to saturate at the quantum resistance h/e at high magnetic field for ν = ± 1 of the x =0.84 device (a) and (b) as well as for ν = +1 of the x =0.88 device (c). In this experiment, we have never observed Shubnikov-de Haas oscillation or quantum Hall plateaus at filling factor ν > 1. This is attributed to low mobility of our films and positive magnetroresistance appearing under low magnetic field. The Quantum Hall plateau with ν = 2 and 3 would have appeared at B = 4 and 5 T. At such a low magnetic field, a sharp increase in Rxx is observed mainly due to the weak antilocalization which is common behavior in this system (3). As a result, ωCτ (ωC is the cyclotron frequency and τ is the scattering time) is lower than 1, meaning appearance of quantum transport is not expected. Above 6 T, Rxx starts to decrease and approaches zero. In case of the electron 2 accumulation side in the x = 0.88 device, Ryx does not reach to h/e at ν = −1 as shown in

Fig.S4d and Rxx does not display a minimum within the maximum available field (B = 14T).

31

Fig.S4 Magnetic field dependence of Rxx (red) and Ryx (blue) at T = 40 mK for x = 0.84 ((a) and (b)) and for x = 0.88 ((c) and (d)) devices. VG is tuned at each QH state. Dashed lines indicate ± h/e2 ~ 25.8 kΩ.

References

1. Zhang, J., et al. Band structure engineering in (Bi1−xSbx)2Te3 ternary topological insulators. Nature Commun. 2, 574 (2012). 2. Yoshimi, R., et al. Dirac electron states formed at the heterointerface between a topological insulator and a conventional semiconductor. Nature Mater. 13, 253-257 (2014). 3. Chen, J., et al. Gate-Voltage Control of Chemical Potential and Weak Antilocalization

in Bi2Se3. Phys. Rev. Lett. 105, 176602 (2010).

32